ferrimagnetic glass-ceramics for cancer ?· ferrimagnetic glass-ceramics for cancer ... fluid...
Post on 24-Aug-2018
Embed Size (px)
FERRIMAGNETIC GLASS-CERAMICS FOR CANCER
O. Bretcanu, S. Ferraris, M. Miola, E. Vern
Materials Science and Chemical Engineering Department, Politecnico di Torino
c-so Duca degli Abruzzi 24, 10129, Turin, Italy
The aim of this work is characterization of bioactive ferrimagnetic glass-ceramics for
magnetic induction hyperthermia. These biomaterials contain different amounts of
magnetite crystals, are bioactive and biocompatible to the human bone osteosarcoma
cells. The surface of these materials was modified in order to bind two different
Keywords: ferrimagnetic, glass-ceramics, hyperthermia, cancer, drug delivery
Magnetic induction hyperthermia is one of the cancer therapies which uses magnetic
materials for the destruction of neoplastic tissue under an alternating magnetic field.
Magnetic field is not absorbed by the living tissue and can be applied to deep regions
into the body. These magnetic materials can be implanted into the tumour and due to
their specific properties, can generate heat under an external alternating magnetic field
(usually by hysteresis loss and eddy current loss), destroying the cancer cells [1, 2]. This
work is focused on the development of bioactive ferrimagnetic glass-ceramics
containing antitumoral drugs for magnetic drug delivery.
Materials and Methods:
Bioactive and biocompatible ferrimagnetic glass-ceramics having the composition in the
system SiO2Na2OCaOP2O5FeOFe2O3 were produced by a traditional melting
method. The theoretical percent of magnetite in these samples is 45wt%. A complete
characterization was performed in terms of morphology and microstructure: scanning
electron microscopy (SEM), X-ray diffraction (XRD), differential thermal analysis
(DTA). Magnetic hysteresis cycle was analysed using a vibrating sample magnetometer
(VSM) with a maximum applied field of 12 kOe (956 kA/m), at room temperature, in
quasi-static conditions. Calorimetric measurements (specific power loss) were carried
out using a magnetic induction furnace, with a magnetic field of 40kA/m and a
frequency of 440 kHz. In vitro bioactivity was analysed by immersing the samples in a
simulated body fluid (SBF) according to Kokubo protocol . After soaking, the
samples were analysed by SEM and XRD. Citotoxicity test was carried out by using
human bone osteosarcoma cells. All the samples were pre-conditioned in culture
medium for 24h before seeding. The surface of these biomaterials was activated in order
to expose hydroxyls groups and to bind two different antitumoral drugs for magnetic
drug delivery (doxorubicin and cisplatinum). The efficiency of the surface modification
and drug release were investigated by contact angle measurements, UV-spectroscopy,
spectrophotometry and X-ray photoemission spectroscopy (XPS).
Results and Discussion:
XRD patterns put in evidence the presence of a unique crystalline phase, magnetite,
embedded in an amorphous residual phase. The XRD pattern of a glass-ceramic sample
is shown in Figure 1. The reflection peaks were identified as magnetite. The DTA
measurements show a glass transition temperature, specific of glass-ceramic materials.
10 15 20 25 30 35 40 45 50 55 60 65 70 75
10 15 20 25 30 35 40 45 50 55 60 65 70 75
Figure 1 XRD spectra of a glass-ceramic sample (M=magnetite crystals)
SEM micrograph of a glass-ceramic sample after chemical etching (with a solution 1:1
HNO3:HF, 5% vol. in distilled water) is shown in Figure 2a. As can be seen, small
interpenetrated columns formed by octahedral crystals with an average size around 1m
are homogeneously distributed in an amorphous matrix. These octahedral crystals are
identified as an iron oxide from EDS measurements (Figure 2b).
The room temperature hysteresis loop of a glass-ceramic sample under a magnetic field
of 12 kOe is shown in Figure 3. The sample exhibits a magnetic behaviour characteristic
of soft magnetic materials. The inset puts in evidence the central part of the hysteresis
loop, emphasising the coercive field and the remanence magnetisation. The specific
power loss of these glass-ceramics is around 20W/g. The hysteresis loss and the specific
power loss are compatible with the temperatures required for hyperthermic treatments
of neoplastic tissues.
Figure 2 a) SEM micrograph of a glass-ceramic sample and b) the EDS spectra of the
area marked on figure 2a.
-15000 -10000 -5000 0 5000 10000 15000-40
Figure 3 Room temperature hysteresis cycle of a glass-ceramic sample
These magnetic glass-ceramics have slow bioactivity kinetics as hydroxylapatite
crystals start to precipitate on the materials surface after 2weeks of soaking in a
simulated body fluid. Citotoxicity tests show that these glass-ceramic materials are
biocompatible to the U2OS osteosarcoma cells. The cells grow healthy and spread in the
culture medium containing magnetic glass-ceramics particles (Figure 4).
Figure 4 U2OS osteosarcoma cells after 24 h in culture medium
XPS and contact angle measurements showed that the samples were efficiently
functionalised and the two drugs can be covalently linked to the glass-ceramic surface.
After one day of uptake at 37C, 777 wt% of doxorubicin and respectively 429 wt%
of cisplatinum are grafted onto the material surface (see Figure 5 a and b). After 1day of
soaking at 37C, the glass-ceramic powders release around 15 wt% of doxorubicin and
about 50 wt% of cisplatinum, respectively (see Figure 5 c and d). The release kinetics is
not uniform, showing irregular up and down peaks. The maximum amount of drugs
released is obtained after 1day of dipping at 37C. The drug release kinetics depends on
the concentration of the drug absorbed on the biomaterial surface and on the type of
solution (water, simulated body fluid).
Figure 5 a) Amounts of doxorubicin (wt%) grafted on samples surface, after one and
two uptake days b) amounts of cisplatinum (wt%) grafted on samples surface, after one
and two uptake days c) amounts of doxorubicin (wt%) released after different times d)
amounts of cisplatinum (wt%) released after different times
Ferrimagnetic glass-ceramics were obtained by a traditional melting method. They
contain magnetite crystals, homogeneously distributed inside the glass matrix. These
biomaterials are both bioactive and biocompatible to human bone osteosarcoma cells.
The surface of these materials can be easily modified, in order to bind specific drugs for
magnetic drug targeting. Further works concerning the drugs release in simulated body
fluid and the study of the drug release kinetics in function of the temperature are in
The authors acknowledge P. Tiberto and P. Allia (National Institute of Metrology,
Turin, Italy) for the magnetic measurements, Roberto Agu and Giorgio Manfredi
(Manfredi S.p.A, Pinerolo, IT) for the calorimetric measurement facilities, I. Marangi,
R. Carbone (European Institute of Oncology, Milan, Italy) for the in vitro tests, C.
Bianchi and A. Naldoni (Dept. Physical Chemistry and Electrochemistry, Milan
University) for XPS measurements and G. Maina (Traumatology Orthopaedics and
Occupational Medicine Department, Turin University) for cisplatinum release test. This
work was partially funded by the Piedmont Region project, Functionalized
ferrimagnetic materials for solid tumours, 2009.
1. Ebisawa Y., Preparation of bioactive and ferrimagnetic glass-ceramics for hyperthermic treatment of cancer, Ph. D thesis, 2000
2. Bretcanu O., Vern E., Cisson M., Tiberto P., Allia P., Journal of Magnetism and Magnetic Materials 2006, 305: 529-533.
3. Kokubo T et al., J. Biomed. Mater. Res. 1990; 24 (3): 331-343
Previous: Previous PaperBack to Programme: Back to ProgrammeBack to Topic: Back to TopicNext: Next Paper